#------------------------------------------------------------------------------
#$Date: 2023-03-26 10:09:57 +0200 (Sun 26 de Mar de 2023) $
#$Revision: 282068 $
#$URL: svn://www.crystallography.net/cod/cif/1/10/10/1101076.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1101076
loop_
_publ_author_name
'Matsushita, Yoshitaka'
'Ueda, Yutaka'
_publ_section_title
;Structure and Physical Properties of 1D Magnetic Chalcogenide,
Jamesonite (FePb4Sb6S14)
;
_journal_name_full               'Inorg. Chem.'
_journal_page_first              7830
_journal_page_last               7838
_journal_paper_doi               10.1021/ic034634t
_journal_volume                  42
_journal_year                    2003
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe Pb4 S14 Sb6'
_chemical_formula_weight         2064.19
_chemical_name_mineral           Jamesonite
_chemical_name_systematic        'Iron tetralead hexaantimony sulfide'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 91.68(8)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   15.750(6)
_cell_length_b                   19.125(3)
_cell_length_c                   4.030(4)
_cell_measurement_temperature    296
_cell_volume                     1213.4(13)
_database_code_amcsd             0018283
_exptl_crystal_density_diffrn    5.651
_cod_depositor_comments
;
The following automatic conversions were performed:

'_cell_measurement_temperature' value '296K' was changed to '296' -
the value should be numeric and without a unit designator.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_original_sg_symbol_H-M      'P 21/a'
_cod_database_code               1101076
loop_
_space_group_symop_operation_xyz
x,y,z
1/2-x,1/2+y,-z
-x,-y,-z
1/2+x,1/2-y,z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Pb1 Pb -0.07429(6) 0.26108(2) 0.0556(1) 0.0211(3) Uani 1.00 d . . .
Pb2 Pb -0.31702(6) 0.35932(3) 0.0341(1) 0.0233(3) Uani 1.00 d . . .
Sb1 Sb 0.1312(1) 0.34110(4) -0.3872(2) 0.0201(4) Uani 1.00 d . . .
Sb2 Sb -0.10379(10) 0.45257(4) -0.3874(2) 0.0153(4) Uani 1.00 d . . .
Sb3 Sb -0.17991(9) 0.06342(4) 0.4116(2) 0.0167(4) Uani 1.00 d . . .
Fe Fe 0.0000 0.0000 0.0000 0.017(1) Uani 1.00 d S . .
S1 S -0.2157(4) 0.4968(2) 0.0268(8) 0.015(1) Uani 1.00 d . . .
S2 S -0.0796(4) 0.1056(1) -0.0108(7) 0.018(1) Uani 1.00 d . . .
S3 S 0.0959(3) 0.0436(1) -0.4770(7) 0.014(1) Uani 1.00 d . . .
S4 S 0.0516(4) 0.2307(1) -0.4319(7) 0.019(1) Uani 1.00 d . . .
S5 S -0.1833(4) 0.3414(1) -0.4505(7) 0.016(1) Uani 1.00 d . . .
S6 S 0.0024(4) 0.3981(1) 0.0466(7) 0.017(1) Uani 1.00 d . . .
S7 S -0.2747(4) 0.2038(2) 0.0747(8) 0.019(1) Uani 1.00 d . . .
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0018283
